Fundamentals of Friction and Wear
of Automobile Brake Materials
Shyam Bahadur, PhD., Fellow ASME, Fellow
University Professor and Professor of
Mechanical Engineering, Iowa State
Outline of Topics
A tribological system
Tribological interactions and wear
Wear of friction materials
Aluminum composite vs. cast iron for
Transfer film and its role
Tribological interactions and wear
Contact between a soft material and a rigid
surface with asperities
Contribution from adhesion and deformation:
Friction force, F = Fadh
Adhesion: van der Waal’s forces, dipole interactions,
hydrogen bonding, electrical charge
Deformation: deformation of polymer asperities –
energy loss due to hysteresis, and grooving
Hysteresis depends upon contact pressure,
deformation rate, and temperature
Viscoelastic effects make friction rate and temperature
Adhesion Component of Friction
Friction force due to adhesion,
A = real area of contact
S = shear strength of adhesion bonds
Sliding velocity-to-strain rate dependence for
area of contact is about 5. This dependence
for shear is 105
The thickness of polymer film affected by
shearing is about a micron thick.
Rolling friction µR and αLE-1/3 vs. temperature for a hard
sphere rolling over a flat PTFE surface. Here αLE-1/3 is
proportional to rolling friction where αL= π tanδ (tanδ is a measure of hysteresis).
Archard’s equation for sliding wear
V/L = K.P/H
V - wear volume L - sliding distance
P – load
H – polymer hardness
K - a proportionality constant. It is a cure-for-all
factor and needs to be determined
Wear volume is not often linearly proportional
Wear volume is not inversely proportional to
Wear Equation for Friction Materials
Wear volume, V = K P
v - sliding velocity
T - time of sliding
P – load
K – proportionality constant
The exponents, a, b and c depend upon the
material combinations and sliding conditions.
S. K. Rhee, Wear, 16 (1970) 431-445. S. K. Rhee, Wear, 18
(1971) 471-477. S. K. Rhee, Wear, 80 (1970) 992-998.
Friction Materials as Composites
Reinforcing fiber materials:
5 - 25 vol.%
Aramid, metal, ceramic, glass, acrylic, and others
Aramid pulp – good filler retention provides green strength for
preform, strong covalent bonding
Ceramic fibers – potassium titanate (K2
-high thermal stability and compatibility with binder material,
high modulus and high strength
Fillers– Barite (BaSO4
Binder – phenolic resin: high hardness and compressive
strength, temperature resistant (300 – 500°
resistant, moldability, wetting capability
Friction Materials: Organic, metallic and
Organic friction materials are the composites of
Polymer as binder resin- phenolic, rubber, cashew
Fibers - organic
Additives - improved strength, thermal expansion and heat
absorption, modification of friction and wear, reduced cost,
Examples of organic friction materials:
Asbestos (also called organic) brake linings with asbestos and
Non-asbestos organic (NAO) brake linings with fibers of
materials other than asbestos, and binder. Fiber material
examples are glass, mineral wool, metal, ceramic, Kevlar, etc.
Also other shapes of reinforcements are used.
Metallic and Carbon Friction Materials
1. Semi-metallic or resin-bonded metallic materials:
Example: Wt.% Fe 65 including 10-25% steel fiber, graphite
15, phenolic binder 10
2. Metallic Friction Materials:
suited for heavy duty
applications, copper or iron based materials sintered with
Examples: solid state sintered bronze with mullite, sintered
iron with graphite.
3. Carbon Friction Materials: high performance (2000°
operating temperature) and light weight material
Example: carbon-carbon friction material which is carbon fiber
bonded with amorphous carbon
Factors affecting the Friction and Wear of
Brake design – disk or drum: loading areas different,
faster cooling in disk brakes
Disk/ Drum and Lining materials composition
Operating temperature range
Exposure to environmental contaminants such as road
dust, local rust debris, moisture, etc.
Friction and Wear Test Machines
Chase Machine – SAE Test J661a
FAST (Friction Assessment and Screening Test) Machine
Block specimen, 6.35 mm2
, rubs on the periphery of a
rotating ring at constant pressure
A pad of friction material loaded by air pressure against the
inside surface of the 279.4 mm diameter drum
Inertial Dynamometer Machine
It use one or more shaft-mounted weights to store energy
which is dissipated by the brake material during testing.
Machines vary in size from laboratory-scale to full-size units.
FMVSS (Federal Motor Vehicle Safety Standard) tests for
brake materials require the use of full-size inertial
Variation of Wear
• Inertial laboratory friction machine
• Variables: load, sliding speed, time, and counterface
• Mating surface of Steel
• Sliding velocity 0.44 – 2.2 m/s, Load 61.2 kg on a surface
area of 280 mm2
Materials A, B, C, D and E: asbestos-reinforced fiction materials
Composition wt.%, bond material 15.00 – 27.71, fillers 69.55
– 81.77, accelerators 0.18 - 1.74, and vulcanizers 0.66 –
Pogosian and Lambarian, Wear of Materials 1977, 547-551,
Wear of asbestos-reinforced friction
materials as a function of normal load,
sliding speed, and time. 61.2 kg, 1.02
m/s, 15 min.
Wear and friction of asbestos-reinforced friction materials sliding
against steel: load 61.2 kg, speed 1.02 m/s, time 15 min.
Wear as a function of temperature for
(vol.%: phenolic binder 15, asbestos fiber 37.5, organic modifier and cashew 36.5, inorganic modifier 11) and
experimental material (potassium titanate + asbestos fibers). Cast iron drum, sliding speed 7.6 m/s, load adjusted for a constant torque of 4.0 kgf-m.
L. Halberstadt, J. A. Mansfield and S. K. Rhee, Wear of
Materials 1977, 560 – 568, ASME, NY
Semilog plots of wear as a function of reciprocal absolute temperature. Arrhenius plots (log W = A – B/T) gave activation energies of 6-10 kcal/mole which indicate thermal decomposition of the phenolic resin binder.
Low temperature region – adhesive and abrasive wear,
High temperature region – thermally activated process
because of the thermal degradation of phenolic resin
binder which is pyrolized and oxidized and finally
worn away as gases or other degradation products.
Oxidation was not the controlling mechanism
because the activation energy is much lower than for
oxidation (30 kcal/mole).
Coefficient of friction as a function of temperature for standard and experimental materials. Note potassium titanate promotes higher friction at high temperatures.
Glass and Carbon Short-Fiber
Reinforced Friction Materials
CFRFM: by Vol.%, Carbon Fiber 34.5, Steel fiber 2.3,
cashew-modified phenolic resin 34.0, phenolic
particles 21.67, BaSO4
CGRFM – material reinforced with glass fibers
Chase machine with cast iron drum 280 mm diameter
rotating at 800 rpm
Thermal damage and pitting observed at high
temperatures: fiber thinning and pullout at low
speeds and temperatures
Fade and Recovery phenomena
wear rate and
P=669 N, V =
Synergistic Effects of Aramid Pulp and
Potassium Titanate Whiskers
Friction material composition Vol.% : Phenolic resin 20,
Barite 45, MoS2
5, Aramid pulp and potassium
titanate used in different proportions
Materials designated as AP-0, AP-0.25, AP-0.75, etc.
(the number indicates the vol.% ratio of aramid in
the total of aramid and potassium titanate)
Pad and disk type of test used
Specific wear rate (x10-5 mm3/Nm) of friction materials.
Sliding conditions: 5 m/s, 1.4 MPa, 100° C, 2.5 km distance.
Comparison of Aluminum-Matrix Composites
with Cast Iron
Blockonring test: Mild 1.5 m/s, 0.4 MPa, Severe
-1.5 m/s, 1.3 MPa
Ring materials – particulate reinforced aluminum
20% SiC-357Al (20SC357)
60% SiC-336Al (55SC336)
Pearlitic gray cast iron
Block material: friction material with non-asbestos
reinforcement, friction modifiers, phenolic binder
Shaw et al., Wear of Materials, ASME 1991, pp. 167-175.
Friction coefficient as a function of time for NAO friction material sliding against Al-composite ring under mild conditions.
Friction coefficient as a function of time for NAO friction material sliding against Al-composite ring under severe conditions.
Wear normalized by energy for NAO friction material sliding against Al composite ring under mild
Wear normalized by energy expended for NAO friction material sliding against Al composite ring under severe conditions.
Transfer Film Studies
Friction material: % by volume
Asbestos 53.3%, organic friction modifier 21.2%, inorganic
friction modifier 0.5%, phenolic resin 25%
Cast iron drum finished to 1.5
rms, rubbing surface
diameter 280 mm
Running conditions: 90 kg load, 300 rpm, 150°
temperature, rubbing surface area 25 mm x 25 mm
Chase machine, two 20 min break-in periods followed by
two 10-min low temperature periods and two 10-min
high temperature periods
SEM micrograph of the cross-section of cast iron drum. It shows transfer film and deformed
cementite platelets in the cast iron subsurface structure.
Scanning Auger Microscopy results. Upper diagram for non-friction location and lower diagram for transfer film. Elements in lower diagram indicate higher C, lower Fe, and the presence of Mg, Si, S and Cl from friction material.